#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:59:59 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179550 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/19/4501916.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4501916
loop_
_publ_author_name
'Parhi, Purnendu'
'Upreti, Shailesh'
'Ramanan, Arunachalam'
_publ_section_title
;
 Crystallization of Calcium Vanadate Solids from Solution: A Metathetic
 Route
;
_journal_issue                   12
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              5078
_journal_paper_doi               10.1021/cg100703h
_journal_volume                  10
_journal_year                    2010
_chemical_formula_moiety         'O28 V10, 14(H2 O), 2(O), 2(N), 2(Ca)'
_chemical_formula_sum            'Ca2 H28 N2 O44 V10'
_chemical_formula_weight         1349.80
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.036(4)
_cell_angle_beta                 102.739(5)
_cell_angle_gamma                110.250(4)
_cell_formula_units_Z            1
_cell_length_a                   9.705(3)
_cell_length_b                   10.231(4)
_cell_length_c                   10.549(3)
_cell_measurement_reflns_used    6680
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      28.26
_cell_measurement_theta_min      2.13
_cell_volume                     955.1(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0269
_diffrn_reflns_av_sigmaI/netI    0.0284
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            9350
_diffrn_reflns_theta_full        25.50
_diffrn_reflns_theta_max         25.50
_diffrn_reflns_theta_min         1.99
_exptl_absorpt_coefficient_mu    2.729
_exptl_absorpt_correction_T_max  0.739
_exptl_absorpt_correction_T_min  0.501
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.347
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             664
_exptl_crystal_size_max          0.324
_exptl_crystal_size_mid          0.213
_exptl_crystal_size_min          0.112
_refine_diff_density_max         1.017
_refine_diff_density_min         -0.900
_refine_diff_density_rms         0.300
_refine_ls_extinction_coef       0.0204(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.257
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     277
_refine_ls_number_reflns         3543
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.257
_refine_ls_R_factor_all          0.0429
_refine_ls_R_factor_gt           0.0381
_refine_ls_shift/su_max          0.010
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0663P)²+0.7505P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1075
_refine_ls_wR_factor_ref         0.1219
_reflns_number_gt                3395
_reflns_number_total             3543
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg100703h_si_001.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4501916
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
V1 V 0.81352(6) 0.69883(6) 0.89471(6) 0.02346(19) Uani 1 1 d .
V2 V 0.51792(6) 0.45850(6) 0.75233(5) 0.02002(19) Uani 1 1 d .
V3 V 0.65461(6) 0.46519(5) 1.05241(5) 0.01732(18) Uani 1 1 d .
V4 V 0.34823(6) 0.22806(6) 0.90803(5) 0.02163(19) Uani 1 1 d .
V5 V 0.47731(6) 0.23998(6) 1.20803(6) 0.02369(19) Uani 1 1 d .
Ca1 Ca 0.84038(8) 0.23341(8) 0.58688(7) 0.0269(2) Uani 1 1 d .
O1 O 0.9829(3) 0.7527(3) 0.8762(3) 0.0350(6) Uani 1 1 d .
O2 O 0.8238(2) 0.5452(2) 1.0177(2) 0.0227(5) Uani 1 1 d .
O3 O 0.7195(3) 0.5437(2) 0.7666(2) 0.0226(5) Uani 1 1 d .
O4 O 0.4655(3) 0.3440(3) 0.6303(2) 0.0291(6) Uani 1 1 d .
O5 O 0.4658(3) 0.6009(2) 0.6791(2) 0.0231(5) Uani 1 1 d .
O6 O 0.5601(2) 0.3415(2) 0.8981(2) 0.0194(5) Uani 1 1 d .
O7 O 0.6720(2) 0.6060(2) 1.1822(2) 0.0179(5) Uani 1 1 d .
O8 O 0.4265(2) 0.4012(2) 1.0685(2) 0.0183(5) Uani 1 1 d .
O9 O 0.6761(3) 0.3440(2) 1.1561(2) 0.0227(5) Uani 1 1 d .
O10 O 0.3000(3) 0.1144(3) 0.7863(3) 0.0338(6) Uani 1 1 d .
O11 O 0.1695(3) 0.1989(2) 0.9538(2) 0.0246(5) Uani 1 1 d .
O12 O 0.4252(3) 0.1435(2) 1.0434(2) 0.0246(5) Uani 1 1 d .
O13 O 0.5298(3) 0.1358(3) 1.3033(3) 0.0369(6) Uani 1 1 d .
O14 O 0.2771(3) 0.1961(3) 1.2082(2) 0.0257(5) Uani 1 1 d .
O1W O 0.5967(3) 0.1384(3) 0.6305(4) 0.0422(7) Uani 1 1 d .
O2W O 1.0966(3) 0.3571(4) 0.6164(3) 0.0489(9) Uani 1 1 d .
O3W O 0.9041(4) 0.0900(3) 0.7608(3) 0.0407(7) Uani 1 1 d .
O4W O 0.7829(5) 0.0144(4) 0.4748(3) 0.0653(11) Uani 1 1 d .
O5W O 0.8892(4) 0.2902(4) 0.3705(3) 0.0537(9) Uani 1 1 d .
O6W O 0.7557(3) 0.4268(3) 0.5341(2) 0.0293(6) Uani 1 1 d .
O7W O 0.8898(3) 0.3664(3) 0.7981(3) 0.0360(7) Uani 1 1 d .
O8W O 0.7142(4) 0.1429(3) 0.9492(3) 0.0490(8) Uani 1 1 d .
N1 N 0.8364(5) 0.7909(5) 0.5747(4) 0.0572(11) Uani 1 1 d .
H1A H 0.6187 0.1290 0.5823 0.045(6) Uiso 1 1 d R
H1B H 0.5482 0.0566 0.6200 0.051(3) Uiso 1 1 d R
H2A H 1.1510 0.3614 0.6753 0.060(18) Uiso 1 1 d R
H2B H 1.1141 0.4179 0.5650 0.070(18) Uiso 1 1 d R
H3A H 0.9686 0.1098 0.7959 0.078(3) Uiso 1 1 d R
H3B H 0.8869 0.0207 0.7404 0.046(2) Uiso 1 1 d R
H4A H 0.7325 0.0468 0.5160 0.061(18) Uiso 1 1 d R
H4B H 0.7988 0.0144 0.4002 0.050(2) Uiso 1 1 d R
H5A H 0.9524 0.2825 0.3322 0.045(2) Uiso 1 1 d R
H5B H 0.8422 0.3054 0.3099 0.062(5) Uiso 1 1 d R
H6A H 0.7678 0.4781 0.5954 0.066(18) Uiso 1 1 d R
H6B H 0.6972 0.4213 0.4775 0.063(18) Uiso 1 1 d R
H7A H 0.9650 0.4090 0.8390 0.043(3) Uiso 1 1 d R
H7B H 0.8524 0.4252 0.8135 0.051(14) Uiso 1 1 d R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 V1 O14 104.42(13) . 2_667
O1 V1 O11 102.94(13) . 2_667
O14 V1 O11 92.52(11) 2_667 2_667
O1 V1 O3 101.05(13) . .
O14 V1 O3 90.99(11) 2_667 .
O11 V1 O3 154.05(11) 2_667 .
O1 V1 O2 99.60(12) . .
O14 V1 O2 155.92(10) 2_667 .
O11 V1 O2 83.70(11) 2_667 .
O3 V1 O2 82.67(10) . .
O1 V1 O8 173.47(12) . 2_667
O14 V1 O8 81.86(10) 2_667 2_667
O11 V1 O8 78.25(9) 2_667 2_667
O3 V1 O8 76.82(9) . 2_667
O2 V1 O8 74.08(9) . 2_667
O1 V1 V5 137.69(10) . 2_667
O14 V1 V5 33.28(8) 2_667 2_667
O11 V1 V5 85.17(8) 2_667 2_667
O3 V1 V5 83.75(7) . 2_667
O2 V1 V5 122.65(7) . 2_667
O8 V1 V5 48.58(6) 2_667 2_667
O1 V1 V4 135.29(11) . 2_667
O14 V1 V4 82.25(8) 2_667 2_667
O11 V1 V4 32.42(7) 2_667 2_667
O3 V1 V4 123.26(7) . 2_667
O2 V1 V4 81.94(7) . 2_667
O8 V1 V4 46.45(5) 2_667 2_667
V5 V1 V4 60.82(2) 2_667 2_667
O4 V2 O3 103.72(12) . .
O4 V2 O5 102.49(12) . .
O3 V2 O5 95.54(11) . .
O4 V2 O6 99.64(12) . .
O3 V2 O6 90.03(10) . .
O5 V2 O6 155.15(10) . .
O4 V2 O7 98.66(12) . 2_667
O3 V2 O7 155.24(10) . 2_667
O5 V2 O7 89.78(10) . 2_667
O6 V2 O7 75.77(9) . 2_667
O4 V2 O8 173.67(11) . 2_667
O3 V2 O8 81.11(9) . 2_667
O5 V2 O8 80.89(10) . 2_667
O6 V2 O8 76.07(9) . 2_667
O7 V2 O8 75.88(9) 2_667 2_667
O4 V2 V5 135.51(10) . 2_667
O3 V2 V5 84.29(8) . 2_667
O5 V2 V5 33.12(7) . 2_667
O6 V2 V5 124.34(7) . 2_667
O7 V2 V5 87.17(7) 2_667 2_667
O8 V2 V5 48.32(6) 2_667 2_667
O2 V3 O9 106.49(12) . .
O2 V3 O6 98.08(11) . .
O9 V3 O6 97.32(11) . .
O2 V3 O7 96.97(11) . .
O9 V3 O7 96.83(11) . .
O6 V3 O7 155.47(10) . .
O2 V3 O8 87.75(10) . 2_667
O9 V3 O8 165.73(10) . 2_667
O6 V3 O8 81.13(9) . 2_667
O7 V3 O8 80.22(9) . 2_667
O2 V3 O8 166.04(10) . .
O9 V3 O8 87.42(10) . .
O6 V3 O8 80.86(9) . .
O7 V3 O8 79.87(9) . .
O8 V3 O8 78.33(10) 2_667 .
O10 V4 O12 102.98(13) . .
O10 V4 O11 102.80(13) . .
O12 V4 O11 95.56(11) . .
O10 V4 O7 101.09(12) . 2_667
O12 V4 O7 153.59(10) . 2_667
O11 V4 O7 89.53(10) . 2_667
O10 V4 O6 100.52(12) . .
O12 V4 O6 88.97(10) . .
O11 V4 O6 154.55(10) . .
O7 V4 O6 76.06(9) 2_667 .
O10 V4 O8 175.11(12) . .
O12 V4 O8 80.14(10) . .
O11 V4 O8 80.48(9) . .
O7 V4 O8 75.16(9) 2_667 .
O6 V4 O8 75.64(9) . .
O10 V4 V1 135.47(10) . 2_667
O12 V4 V1 83.50(8) . 2_667
O11 V4 V1 32.93(7) . 2_667
O7 V4 V1 86.95(7) 2_667 2_667
O6 V4 V1 123.81(7) . 2_667
O8 V4 V1 48.19(6) . 2_667
O13 V5 O14 104.11(13) . .
O13 V5 O5 101.57(13) . 2_667
O14 V5 O5 91.87(11) . 2_667
O13 V5 O12 102.66(14) . .
O14 V5 O12 91.07(11) . .
O5 V5 O12 154.08(11) 2_667 .
O13 V5 O9 99.59(12) . .
O14 V5 O9 156.29(10) . .
O5 V5 O9 83.72(10) 2_667 .
O12 V5 O9 83.30(10) . .
O13 V5 O8 174.20(12) . .
O14 V5 O8 81.67(9) . .
O5 V5 O8 77.53(9) 2_667 .
O12 V5 O8 77.44(9) . .
O9 V5 O8 74.63(9) . .
O13 V5 V1 137.21(11) . 2_667
O14 V5 V1 33.10(7) . 2_667
O5 V5 V1 84.84(7) 2_667 2_667
O12 V5 V1 83.66(8) . 2_667
O9 V5 V1 123.19(7) . 2_667
O8 V5 V1 48.57(5) . 2_667
O13 V5 V2 133.86(11) . 2_667
O14 V5 V2 82.05(8) . 2_667
O5 V5 V2 32.35(7) 2_667 2_667
O12 V5 V2 123.14(7) . 2_667
O9 V5 V2 81.87(7) . 2_667
O8 V5 V2 45.71(5) . 2_667
V1 V5 V2 60.857(19) 2_667 2_667
O2W Ca1 O4W 108.45(15) . .
O2W Ca1 O1W 160.59(13) . .
O4W Ca1 O1W 86.19(14) . .
O2W Ca1 O6W 97.14(11) . .
O4W Ca1 O6W 132.56(11) . .
O1W Ca1 O6W 80.98(10) . .
O2W Ca1 O3W 88.05(11) . .
O4W Ca1 O3W 76.46(12) . .
O1W Ca1 O3W 82.99(11) . .
O6W Ca1 O3W 145.21(11) . .
O2W Ca1 O5W 72.47(11) . .
O4W Ca1 O5W 75.53(13) . .
O1W Ca1 O5W 124.84(12) . .
O6W Ca1 O5W 75.17(11) . .
O3W Ca1 O5W 138.32(12) . .
O2W Ca1 O7W 80.26(11) . .
O4W Ca1 O7W 147.29(12) . .
O1W Ca1 O7W 80.62(11) . .
O6W Ca1 O7W 74.71(9) . .
O3W Ca1 O7W 72.32(11) . .
O5W Ca1 O7W 135.97(12) . .
O2W Ca1 H1A 173.7 . .
O4W Ca1 H1A 75.4 . .
O1W Ca1 H1A 13.3 . .
O6W Ca1 H1A 83.3 . .
O3W Ca1 H1A 88.1 . .
O5W Ca1 H1A 113.6 . .
O7W Ca1 H1A 93.9 . .
O2W Ca1 H2A 12.3 . .
O4W Ca1 H2A 109.9 . .
O1W Ca1 H2A 150.0 . .
O6W Ca1 H2A 103.5 . .
O3W Ca1 H2A 76.8 . .
O5W Ca1 H2A 84.5 . .
O7W Ca1 H2A 72.3 . .
H1A Ca1 H2A 161.9 . .
O2W Ca1 H2B 16.2 . .
O4W Ca1 H2B 111.3 . .
O1W Ca1 H2B 162.1 . .
O6W Ca1 H2B 84.1 . .
O3W Ca1 H2B 104.2 . .
O5W Ca1 H2B 59.6 . .
O7W Ca1 H2B 85.9 . .
H1A Ca1 H2B 166.9 . .
H2A Ca1 H2B 28.0 . .
O2W Ca1 H4A 127.6 . .
O4W Ca1 H4A 19.7 . .
O1W Ca1 H4A 66.5 . .
O6W Ca1 H4A 124.6 . .
O3W Ca1 H4A 75.2 . .
O5W Ca1 H4A 87.9 . .
O7W Ca1 H4A 135.9 . .
H1A Ca1 H4A 55.9 . .
H2A Ca1 H4A 127.3 . .
H2B Ca1 H4A 131.0 . .
V3 O2 V1 110.22(12) . .
V2 O3 V1 114.05(12) . .
V2 O5 V5 114.53(12) . 2_667
V3 O6 V2 106.81(11) . .
V3 O6 V4 108.22(11) . .
V2 O6 V4 100.16(10) . .
V3 O7 V4 108.23(11) . 2_667
V3 O7 V2 107.64(10) . 2_667
V4 O7 V2 100.59(10) 2_667 2_667
V3 O8 V3 101.67(9) 2_667 .
V3 O8 V2 93.15(9) 2_667 2_667
V3 O8 V2 93.79(8) . 2_667
V3 O8 V4 93.56(8) 2_667 .
V3 O8 V4 92.70(8) . .
V2 O8 V4 169.54(11) 2_667 .
V3 O8 V1 87.95(8) 2_667 2_667
V3 O8 V1 170.30(11) . 2_667
V2 O8 V1 86.87(8) 2_667 2_667
V4 O8 V1 85.36(7) . 2_667
V3 O8 V5 170.79(11) 2_667 .
V3 O8 V5 87.54(8) . .
V2 O8 V5 85.97(8) 2_667 .
V4 O8 V5 86.12(8) . .
V1 O8 V5 82.85(8) 2_667 .
V3 O9 V5 110.42(11) . .
V4 O11 V1 114.65(12) . 2_667
V4 O12 V5 115.19(13) . .
V1 O14 V5 113.61(13) 2_667 .
Ca1 O1W H1A 49.8 . .
Ca1 O1W H1B 122.6 . .
H1A O1W H1B 85.9 . .
Ca1 O2W H2A 123.7 . .
Ca1 O2W H2B 112.1 . .
H2A O2W H2B 120.4 . .
Ca1 O3W H3A 119.2 . .
Ca1 O3W H3B 114.5 . .
H3A O3W H3B 106.2 . .
Ca1 O4W H4A 47.6 . .
Ca1 O4W H4B 117.4 . .
H4A O4W H4B 138.0 . .
Ca1 O5W H5A 133.6 . .
Ca1 O5W H5B 132.2 . .
H5A O5W H5B 93.0 . .
Ca1 O6W H6A 114.1 . .
Ca1 O6W H6B 120.8 . .
H6A O6W H6B 119.6 . .
Ca1 O7W H7A 126.2 . .
Ca1 O7W H7B 126.8 . .
H7A O7W H7B 92.0 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
V1 O1 1.600(3) .
V1 O14 1.828(2) 2_667
V1 O11 1.854(2) 2_667
V1 O3 1.905(2) .
V1 O2 2.054(2) .
V1 O8 2.318(2) 2_667
V1 V5 3.0672(10) 2_667
V1 V4 3.0993(10) 2_667
V2 O4 1.608(2) .
V2 O3 1.816(2) .
V2 O5 1.821(2) .
V2 O6 2.007(2) .
V2 O7 2.007(2) 2_667
V2 O8 2.221(2) 2_667
V2 V5 3.0959(11) 2_667
V3 O2 1.684(2) .
V3 O9 1.690(2) .
V3 O6 1.905(2) .
V3 O7 1.926(2) .
V3 O8 2.103(2) 2_667
V3 O8 2.126(2) .
V4 O10 1.605(3) .
V4 O12 1.823(2) .
V4 O11 1.828(2) .
V4 O7 1.994(2) 2_667
V4 O6 2.007(2) .
V4 O8 2.254(2) .
V4 V1 3.0993(10) 2_667
V5 O13 1.599(3) .
V5 O14 1.837(2) .
V5 O5 1.859(2) 2_667
V5 O12 1.874(3) .
V5 O9 2.049(2) .
V5 O8 2.318(2) .
V5 V1 3.0672(10) 2_667
V5 V2 3.0960(11) 2_667
Ca1 O2W 2.316(3) .
Ca1 O4W 2.360(3) .
Ca1 O1W 2.375(3) .
Ca1 O6W 2.413(3) .
Ca1 O3W 2.457(3) .
Ca1 O5W 2.461(3) .
Ca1 O7W 2.474(3) .
Ca1 H1A 2.0333 .
Ca1 H2A 2.7747 .
Ca1 H2B 2.7336 .
Ca1 H4A 1.8891 .
O5 V5 1.859(2) 2_667
O7 V4 1.994(2) 2_667
O7 V2 2.008(2) 2_667
O8 V3 2.103(2) 2_667
O8 V2 2.221(2) 2_667
O8 V1 2.318(2) 2_667
O11 V1 1.854(2) 2_667
O14 V1 1.828(2) 2_667
O1W H1A 0.6125 .
O1W H1B 0.7992 .
O2W H2A 0.7118 .
O2W H2B 0.8225 .
O3W H3A 0.6166 .
O3W H3B 0.6922 .
O4W H4A 0.8623 .
O4W H4B 0.8352 .
O5W H5A 0.8308 .
O5W H5B 0.7495 .
O6W H6A 0.7943 .
O6W H6B 0.7140 .
O7W H7A 0.7411 .
O7W H7B 0.8347 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O9 V3 O2 V1 -178.75(10) . .
O6 V3 O2 V1 81.10(13) . .
O7 V3 O2 V1 -79.47(13) . .
O8 V3 O2 V1 0.39(12) 2_667 .
O8 V3 O2 V1 -3.5(5) . .
O1 V1 O2 V3 -178.71(13) . .
O14 V1 O2 V3 -2.9(3) 2_667 .
O11 V1 O2 V3 79.17(13) 2_667 .
O3 V1 O2 V3 -78.68(13) . .
O8 V1 O2 V3 -0.36(11) 2_667 .
V5 V1 O2 V3 -0.96(16) 2_667 .
V4 V1 O2 V3 46.54(11) 2_667 .
O4 V2 O3 V1 174.56(13) . .
O5 V2 O3 V1 70.23(14) . .
O6 V2 O3 V1 -85.51(13) . .
O7 V2 O3 V1 -31.4(3) 2_667 .
O8 V2 O3 V1 -9.62(12) 2_667 .
V5 V2 O3 V1 39.03(11) 2_667 .
O1 V1 O3 V2 -176.96(14) . .
O14 V1 O3 V2 -72.06(14) 2_667 .
O11 V1 O3 V2 25.8(3) 2_667 .
O2 V1 O3 V2 84.64(13) . .
O8 V1 O3 V2 9.35(11) 2_667 .
V5 V1 O3 V2 -39.51(11) 2_667 .
V4 V1 O3 V2 9.32(16) 2_667 .
O4 V2 O5 V5 -176.04(13) . 2_667
O3 V2 O5 V5 -70.64(14) . 2_667
O6 V2 O5 V5 31.5(3) . 2_667
O7 V2 O5 V5 85.14(13) 2_667 2_667
O8 V2 O5 V5 9.41(12) 2_667 2_667
O2 V3 O6 V2 -72.41(12) . .
O9 V3 O6 V2 179.69(11) . .
O7 V3 O6 V2 54.9(3) . .
O8 V3 O6 V2 14.02(10) 2_667 .
O8 V3 O6 V2 93.51(11) . .
O2 V3 O6 V4 -179.47(11) . .
O9 V3 O6 V4 72.63(12) . .
O7 V3 O6 V4 -52.1(3) . .
O8 V3 O6 V4 -93.04(11) 2_667 .
O8 V3 O6 V4 -13.55(10) . .
O4 V2 O6 V3 171.26(12) . .
O3 V2 O6 V3 67.33(12) . .
O5 V2 O6 V3 -36.0(3) . .
O7 V2 O6 V3 -92.17(11) 2_667 .
O8 V2 O6 V3 -13.50(10) 2_667 .
V5 V2 O6 V3 -15.77(13) 2_667 .
O4 V2 O6 V4 -76.04(13) . .
O3 V2 O6 V4 -179.96(10) . .
O5 V2 O6 V4 76.7(3) . .
O7 V2 O6 V4 20.53(9) 2_667 .
O8 V2 O6 V4 99.20(10) 2_667 .
V5 V2 O6 V4 96.94(9) 2_667 .
O10 V4 O6 V3 -170.08(13) . .
O12 V4 O6 V3 -67.07(12) . .
O11 V4 O6 V3 33.7(3) . .
O7 V4 O6 V3 90.97(11) 2_667 .
O8 V4 O6 V3 13.02(10) . .
V1 V4 O6 V3 14.40(14) 2_667 .
O10 V4 O6 V2 78.30(14) . .
O12 V4 O6 V2 -178.68(10) . .
O11 V4 O6 V2 -77.9(3) . .
O7 V4 O6 V2 -20.65(9) 2_667 .
O8 V4 O6 V2 -98.59(10) . .
V1 V4 O6 V2 -97.22(9) 2_667 .
O2 V3 O7 V4 72.29(12) . 2_667
O9 V3 O7 V4 179.91(11) . 2_667
O6 V3 O7 V4 -55.2(3) . 2_667
O8 V3 O7 V4 -14.21(10) 2_667 2_667
O8 V3 O7 V4 -93.97(10) . 2_667
O2 V3 O7 V2 -179.79(11) . 2_667
O9 V3 O7 V2 -72.17(12) . 2_667
O6 V3 O7 V2 52.7(3) . 2_667
O8 V3 O7 V2 93.72(11) 2_667 2_667
O8 V3 O7 V2 13.96(10) . 2_667
O2 V3 O8 V3 4.0(4) . 2_667
O9 V3 O8 V3 179.40(11) . 2_667
O6 V3 O8 V3 -82.75(10) . 2_667
O7 V3 O8 V3 81.99(10) . 2_667
O8 V3 O8 V3 -0.001(1) 2_667 2_667
O2 V3 O8 V2 -90.0(4) . 2_667
O9 V3 O8 V2 85.39(10) . 2_667
O6 V3 O8 V2 -176.76(10) . 2_667
O7 V3 O8 V2 -12.02(9) . 2_667
O8 V3 O8 V2 -94.01(10) 2_667 2_667
O2 V3 O8 V4 98.2(4) . .
O9 V3 O8 V4 -86.40(10) . .
O6 V3 O8 V4 11.44(9) . .
O7 V3 O8 V4 176.19(9) . .
O8 V3 O8 V4 94.20(9) 2_667 .
O2 V3 O8 V5 -175.8(4) . .
O9 V3 O8 V5 -0.40(10) . .
O6 V3 O8 V5 97.44(9) . .
O7 V3 O8 V5 -97.82(9) . .
O8 V3 O8 V5 -179.81(12) 2_667 .
O12 V4 O8 V3 -177.72(10) . 2_667
O11 V4 O8 V3 -80.31(10) . 2_667
O7 V4 O8 V3 11.74(8) 2_667 2_667
O6 V4 O8 V3 90.82(9) . 2_667
V1 V4 O8 V3 -87.65(8) 2_667 2_667
O12 V4 O8 V3 80.40(10) . .
O11 V4 O8 V3 177.81(10) . .
O7 V4 O8 V3 -90.14(9) 2_667 .
O6 V4 O8 V3 -11.07(8) . .
V1 V4 O8 V3 170.47(11) 2_667 .
O12 V4 O8 V2 -47.9(6) . 2_667
O11 V4 O8 V2 49.5(6) . 2_667
O7 V4 O8 V2 141.5(6) 2_667 2_667
O6 V4 O8 V2 -139.4(6) . 2_667
V1 V4 O8 V2 42.1(5) 2_667 2_667
O12 V4 O8 V1 -90.07(9) . 2_667
O11 V4 O8 V1 7.34(9) . 2_667
O7 V4 O8 V1 99.39(9) 2_667 2_667
O6 V4 O8 V1 178.46(9) . 2_667
O12 V4 O8 V5 -6.94(9) . .
O11 V4 O8 V5 90.46(9) . .
O7 V4 O8 V5 -177.49(9) 2_667 .
O6 V4 O8 V5 -98.41(9) . .
V1 V4 O8 V5 83.13(7) 2_667 .
O14 V5 O8 V3 -179.04(9) . .
O5 V5 O8 V3 87.17(9) 2_667 .
O12 V5 O8 V3 -86.06(10) . .
O9 V5 O8 V3 0.35(8) . .
V1 V5 O8 V3 -178.68(10) 2_667 .
V2 V5 O8 V3 93.98(8) 2_667 .
O14 V5 O8 V2 86.99(9) . 2_667
O5 V5 O8 V2 -6.81(9) 2_667 2_667
O12 V5 O8 V2 179.96(10) . 2_667
O9 V5 O8 V2 -93.63(9) . 2_667
V1 V5 O8 V2 87.34(7) 2_667 2_667
O14 V5 O8 V4 -86.16(10) . .
O5 V5 O8 V4 -179.95(10) 2_667 .
O12 V5 O8 V4 6.82(9) . .
O9 V5 O8 V4 93.22(9) . .
V1 V5 O8 V4 -85.80(7) 2_667 .
V2 V5 O8 V4 -173.14(10) 2_667 .
O14 V5 O8 V1 -0.35(9) . 2_667
O5 V5 O8 V1 -94.15(9) 2_667 2_667
O12 V5 O8 V1 92.62(9) . 2_667
O9 V5 O8 V1 179.03(9) . 2_667
V2 V5 O8 V1 -87.34(7) 2_667 2_667
O2 V3 O9 V5 179.34(10) . .
O6 V3 O9 V5 -79.95(13) . .
O7 V3 O9 V5 79.96(12) . .
O8 V3 O9 V5 2.9(5) 2_667 .
O8 V3 O9 V5 0.49(11) . .
O13 V5 O9 V3 -179.94(14) . .
O14 V5 O9 V3 1.1(3) . .
O5 V5 O9 V3 -79.21(13) 2_667 .
O12 V5 O9 V3 78.30(13) . .
O8 V5 O9 V3 -0.46(11) . .
V1 V5 O9 V3 0.41(16) 2_667 .
V2 V5 O9 V3 -46.65(11) 2_667 .
O10 V4 O11 V1 173.61(14) . 2_667
O12 V4 O11 V1 68.92(15) . 2_667
O7 V4 O11 V1 -85.12(13) 2_667 2_667
O6 V4 O11 V1 -30.4(3) . 2_667
O8 V4 O11 V1 -10.08(12) . 2_667
O10 V4 O12 V5 -174.35(14) . .
O11 V4 O12 V5 -69.82(15) . .
O7 V4 O12 V5 30.4(3) 2_667 .
O6 V4 O12 V5 85.09(14) . .
O8 V4 O12 V5 9.49(13) . .
V1 V4 O12 V5 -39.12(12) 2_667 .
O13 V5 O12 V4 176.63(14) . .
O14 V5 O12 V4 71.92(15) . .
O5 V5 O12 V4 -24.6(3) 2_667 .
O9 V5 O12 V4 -84.99(14) . .
O8 V5 O12 V4 -9.31(12) . .
V1 V5 O12 V4 39.59(12) 2_667 .
V2 V5 O12 V4 -9.28(17) 2_667 .
O13 V5 O14 V1 -179.98(15) . 2_667
O5 V5 O14 V1 77.59(14) 2_667 2_667
O12 V5 O14 V1 -76.65(14) . 2_667
O9 V5 O14 V1 -1.0(4) . 2_667
O8 V5 O14 V1 0.49(13) . 2_667
V2 V5 O14 V1 46.68(12) 2_667 2_667
